The inhibitory effect of di-imine-SB namely ((N1Z, N4E)-N1, N4-bis (4 (dimethylamino) benzylidene) butane 1,4-diamine) on X65-steel in 1 M HCl has been investigated experimentally and theoretically. The electrochemical impedance spectroscopy (EIS), potentiodynamic polarization (PDP), and weight loss outcomes display the anticorrosion properties of “di-imine- SB”. The inhibitory efficiency exceeds 90% at the optimal concentration of 1 × 10–3M “di-imine- SB”. The metal surface was examined further using scanning electron microscope (SEM) and energy dispersive X-ray (EDX). The effectiveness of the di-imine-SB is returned into its adsorption on X65-steel surface and found in agreement with Langmuir adsorption isotherm. According to the standard Gibbs free energy of adsorption\documentclass[12pt]{minimal}
				\usepackage{amsmath}
				\usepackage{wasysym} 
				\usepackage{amsfonts} 
				\usepackage{amssymb} 
				\usepackage{amsbsy}
				\usepackage{mathrsfs}
				\usepackage{upgreek}
				\setlength{\oddsidemargin}{-69pt}
				\begin{document}$$({\Delta G}_{ads}^{^\circ })$$\end{document}(ΔGads∘), di-imine-SB adsorption tends to be chemical rather than physical, it increases the activation energy (\documentclass[12pt]{minimal}
				\usepackage{amsmath}
				\usepackage{wasysym} 
				\usepackage{amsfonts} 
				\usepackage{amssymb} 
				\usepackage{amsbsy}
				\usepackage{mathrsfs}
				\usepackage{upgreek}
				\setlength{\oddsidemargin}{-69pt}
				\begin{document}$${\mathrm{E}}_{a}$$\end{document}Ea) of metal dissolution reaction and makes it hard to occur. The PDP data suggested anodic and cathodic type of the di-imine-SB inhibitor. Meanwhile, increasing the resistance of X65-steel to 301 Ω cm2after adding 1 mM of di-imine-SB confirms its protective effect. Whereas, the positive value of the fraction of electron transference (ΔN, 0.746), confirms the affinity of di-imine-SB to share electrons to the partially filed 3d-orbital of Fe forming strong protective film over X65-steel surface. Aided by Monte Carlo (MC) simulation, the calculated adsorption energy (Eads) suggests excessive adsorption affinity of di-imine-SB on metal surface over the corrosive chlorides and hydronium ions. A good correlation between the theoretical hypothesis and the experimental inhibition efficiency has been achieved. The comparative study showed the superior of the di-imine-SB as potential corrosion inhibitor compared with those reported before. Finally, global reactivity descriptors; electron affinity (A), ionization potential (I), electronegativity (χ), dipole moment (µ), global hardness (\documentclass[12pt]{minimal}
				\usepackage{amsmath}
				\usepackage{wasysym} 
				\usepackage{amsfonts} 
				\usepackage{amssymb} 
				\usepackage{amsbsy}
				\usepackage{mathrsfs}
				\usepackage{upgreek}
				\setlength{\oddsidemargin}{-69pt}
				\begin{document}$$\eta$$\end{document}η), electrophilicity index and, Fukui indices were also calculated and found well correlated to the reactivity of di-imine-SB.